6 H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003Fig. 3 Methods for achieving self-compactability. Fig. 5 Comparison of mix-proportioning of SCC with other types of conventional concrete.compactability (Fig. 3) (1995): ratios of the coarse aggregate volume to its solid volume (G/Glim) of each type of concrete are shown in Fig. 6. (1) Limited aggregate content The degree of packing of coarse aggregate in SCC is (2) Low water-powder ratio approximately 50% to reduce the interaction between (3) Use of superplasticizer coarse aggregate particles when the concrete deforms. In addition, the ratios of fine aggregate volume to solid The frequency of collision and contact between aggre- volume (S/Slim) in the mortar are shown in the samegate particles can increase as the relative distance figure. The degree of packing of fine aggregate in SCCbetween the particles decreases and then internal stress mortar is approximately 60% so that shear deformabilitycan increase when concrete is deformed, particularly when the concrete deforms may be limited. On thenear obstacles. Research has found that the energy other hand, the viscosity of the paste in SCC is the high-required for flowing is consumed by the increased inter- est among the various types of concrete due to its lowestnal stress, resulting in blockage of aggregate particles. water-powder ratio (Fig. 7). This characteristic isLimiting the coarse aggregate content, whose energy effective in inhibiting segregation.consumption is particularly intense, to a level lower thannormal is effective in avoiding this kind of blockage. Highly viscous paste is also required to avoid theblockage of coarse aggregate when concrete flowsthrough obstacles (Fig. 4). When concrete is deformed,paste with a high viscosity also prevents localizedincreases in internal stress due to the approach of coarseaggregate particles. High deformability can be achievedonly by the employment of a superplasticizer, keepingthe water-powder ratio to a very low value. The mix proportioning of self-compacting concrete isshown and compared with those of normal concrete andRCD (Roller Compacted concrete for Dams) concrete(Fig. 5). The aggregate content is smaller than conven-tional concrete that requires vibrating compaction. The Fig. 6 Degree of aggregate’s compaction-Coarse aggregate in concrete and fine aggregate in mortar. Fig. 7 Relationship between paste volume and water-Fig. 4 Mechanism for achieving self-compactability. powder ratio.
H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 7 open the center gate680 mm obstacle 200 280 height Fig. 8 U-flow test. Fig. 9 Box test. Fig. 11 V-funnel. There are three purposes for self-compactability tests Flow and funnel tests for mortar or paste have been relating to practical purposes. proposed to characterize materials used in self- compacting concrete, e.g. powder material, sand, and Test (1): To check whether or not the concrete is super-plasticizer. Testing methods for the mortar prop- self-compactable for the structure erties were also proposed and the indices for Test (2): To adjust the mix proportion when self- deformability and viscosity were also defined as G m and compactability is not sufficient Rm (Figs. 12 and 13). Test (3): To characterize materials G m = ( d1 d2 - d02 )/d02, As Test (1), the so-called U-flow test or Box test is d1, d2: measured flow diameter; recommended (Figs. 8, 9 and 10). The U-flow test was developed by the Taisei Group (Hayakawa 1993). In d0: flow cone diameter this test, the degree of compactability can be indicated Rm = 10/t, by the height that the concrete reaches after flowing t (sec): measured time (sec) for mortar to flow through an obstacle. Concrete with a filling height of through the funnel over 300 mm can be judged as self-compacting. The Box-test is more suitable for detecting concrete with A larger G m indicates higher deformability and a higher possibility of segregation between coarse aggre- smaller Rm indicates higher viscosity. Characterizing gate and mortar. methods for materials were proposed using the G m and If the concrete is judged to be having insufficient self- Rm indices. compactability through test (1), the cause has to be detected quantitatively so that the mix proportion can be adjusted. Slump-flow and funnel tests (Fig. 11) have been proposed for testing deformability and viscosity, respectively, and the indices were also defined as G c and Rc. G c =(Sfl1 Sfl2 - Sfl02)/Sfl02, Sfl1,Sfl2: measured flow diameter; Sfl0: Slump cone diameter Rc = 10/t, t (sec): measured time (sec) for concrete to flow through the funnel Fig. 12 Mortar flow test Fig. 10 Obstacles employed in Box test: R2 (Left) and R1 (Right). Fig. 13 Mortar funnel test.
8 H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 2.2 Factors of self-compactability in terms of Sufficient deformability of the mortar phase in concrete testing results is required so that concrete can be compacted into struc- The factors making up self-compactability were tures by its self-weight without need for vibrating com- described in terms of the test results for fresh concrete paction. In addition, moderate viscosity as well as and mortar below. deformability of the mortar phase is required so that the relative displacement between coarse aggregate parti- (1) Influence of coarse aggregate depending on cles in front of obstacles when concrete is to flow spacing size around such obstacles can be reduced and then segrega- It is not always possible to predict the degree of com- tion between coarse aggregate and mortar can be inhib- paction into a structure by using the test result on the ited. The necessity for viscosity was confirmed by degree of compaction of the concrete into another struc- Hashimoto’s visualization test. ture, since the maximum size of coarse aggregate is The indices for mortar deformability G m and viscosity close to the minimum spacing between the reinforcing Rm were proposed by using mortar flow and funnel test bars of the structure. For example, the relationship results. The relationship between mortar deformability between coarse aggregate content in concrete and the and viscosity and the self-compactability of fresh con- filling height of the Box-type test, which the standard crete is shown assuming a fixed coarse aggregate con- index for self-compactability of fresh concrete, is shown tent (Fig. 15). The existence of an optimum combina- in Figs. 14 and 15. The relationship between the filling tion of deformability and viscosity of mortar for height through obstacle R1 and that through R2 varied achieving self-compactability of fresh concrete was depending on the coarse aggregate content. That test demonstrated. result shows that the influence of coarse aggregate on the flowability of fresh concrete largely depends on the (3) Role of mortar as solid particles size of the spacing of the obstacle. It can be said that In addition to its role as a liquid mentioned above, mor- the self-compactability of fresh concrete has to be dis- tar also plays a role as solid particles. This property is cussed in terms of solid particles as well as in terms of so-called “pressure transferability”, which can be appar- liquid. ent when the coarse aggregate particles approach each other and mortar in between coarse aggregate particles (2) Role of mortar as fluid in flowability of fresh is subjected to normal stress (Fig. 16). The degree of concrete the decrease in the shear deformability of the mortar largely depends on the physical characteristics of the 400 solid particles in the mortar (Fig. 17) (Nagamoto 1997).Filling height of Box-test (mm) For example, the difference in the relationships 300 between the funnel speeds of mortar and concrete due to 200 t :mortar’s shear s : normal stress Obstacle R2 (3 hours) resistance 100 t steel plate Obstacle R1 (5 hours) s mortar 0 steel plate 250 300 350 Unit coarse aggregate content (litter/m3) Fig. 14 Influence of coarse aggregate content on self- Fig. 16 Normal stress generated in mortar due to compactability. approaching coarse aggregate particles. Fig. 17 Degree of increase in shear deform resistance t Fig. 15 Relationship between mortar’s flowability and due to s depending on physical characteristics of solid self-compctability of fresh concrete. particles.
H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 9Fig. 18 Relationship between mortar’s and concrete’s Fig. 21 Unique relationship between Rcs/Rm andflowability (V65 funnel). degree of self-compactability.differences in the fine aggregate content in mortar are Rcs/Rm are shown in Fig. 20. The difference in theshown in Fig. 18. It was found that the relationship characteristics of the solid particles in mortar can bebetween the flowability of mortar and concrete cannot reflected by the value of Rcs/Rm. The relationshipalways be unique due to differences in the characteris- between Rcs/Rm and the filling height of the Box-typetics of the solid particles in the mortar, even if the char- test, which is the index for self-compactability of freshacteristics of the coarse aggregate and its content in con- concrete, is shown in Fig. 21. It was found that thecrete are constant. relationship was unique despite the differences in the A simple evaluation method for the stress transferabil- fine aggregate content in mortar or the characteristics ofity of mortar was proposed by using the ratio of the fun- sand or powder particles.nel speed of concrete with glass beads as the standardcoarse aggregate (Rcs) to the speed of mortar (Rm) (Fig. (4) Influence of coarse aggregate -Content, shape19) (Ouchi 2000). The higher stress transferability cor- and grading-responds to the smaller value of Rcs/Rm. The relation- T h e i n f lu e n ce o f c o a r se a g g r eg a t e o n t h e s el f -ships between fine aggregate content in mortar and compactability of fresh concrete, especially flowability through obstacles, can be equal despite the shape of the coarse aggregate particles’ shape as long as the ratio of coarse aggregate content to its solid volume in concrete is the same (Fig. 22) (Matsuo, et al., 1994). However, the influence of the grading of coarse aggregate has also to be considered if the spacing of the obstacles is very close to the maximum size coarse aggregate. For exam- ple, the relationships between the size of the concrete funnel’s outlet and the flow speed through it depends onFig. 19 A Simple Evaluation Method for Stress Transfer-ability of Fresh Mortar.Fig. 20 Relationships between fine aggregate content inmortar and Rcs/Rm[1: OPC+Crushed Sand(CS), 2: Fly Ash (FA)+CS, 3: Fig. 22 Unique relationship between ratio of coarseFA+River Sand(RS), 4: OPC + RS, 5: OPC+Land aggregate content to its solid volume in concrete despiteSand(LS)]. difference in gravel shape.
10 H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 investigations to establish the following items have been carried out mainly at the University of Tokyo since the development of the prototype. (1) Self-compactability testing method (2) Mix-design method (3) Acceptance testing method at job site (4) New type of powder or admixture suitable for self-compacting concrete Of those items, (1) has already been mentioned in this paper. (2), (3) and (4) are described below Fig. 23 V-funnel. 3.2 Mix-design method (1) Rational mix-design methodthe fineness modulus of coarse aggregate FM even if the Self-compactability can be largely affected by the char-property of the mortar phase is the same (Figs. 23 and acteristics of materials and the mix proportion. A ratio-24). It was found out that the flow speed of concrete nal mix-design method for self-compacting concretethrough a funnel with an outlet width of 55 mm was using a variety of materials is necessary. Okamura andlargely influenced by the grading of the coarse aggre- Ozawa (1995) have proposed a simple mix proportion-gate. ing system assuming general supply from ready-mixed concrete plants. The coarse and fine aggregate contents3. State of the art on Self-Compacting Con- are fixed so that self-compactability can be achievedcrete easily by adjusting the water-powder ratio and superplasticizer dosage only.3.1 Current status of Self-Compacting ConcreteSelf-compacting concrete has been used as a “special (1) The coarse aggregate content in concrete is fixedconcrete” only in large general construction companies at 50% of the solid volume.in Japan. In order for self-compacting concrete to be (2) The fine aggregate content is fixed at 40% of theused as a standard concrete rather than a special one, mortar volume.new systems for its design, manufacturing and construc- (3) The water-powder ratio in volume is assumed astion of self-compacting concrete need to be established. 0.9 to 1.0, depending on the properties of the powder.Various committee activities on self-compacting con- (4) The superplasticizer dosage and the final water-crete have been carried out as a result. powder ratio are determined so as to ensure self- Among them, a system by which the ready-mixed compactability.concrete industry can produce self-compacting concreteas a normal concrete would seem the most effective In the mix proportioning of conventional concrete, thesince, in Japan, as much as 70% of all concrete is pro- water-cement ratio is fixed at first from the viewpoint ofduced by the ready-mixed concrete industry. Assuming obtaining the required strength. With self-compactinga general supply from ready-mixed concrete plants, concrete, however, the water-powder ratio has to be decided taking into account self-compactability because self-compactability is very sensitive to this ratio. In most cases, the required strength does not govern the water-cement ratio because the water-powder ratio is small enough for obtaining the required strength for ordinary structures unless most of the powder materials in use is not reactive. The mortar or paste in self-compacting concrete requires high viscosity as well as high deformability. This can be achieved by the employment of a superplasticizer, which results in a low water-powder ratio for high deformability. (2) Adjustment of water-powder ratio and super- plasticizer dosage The characteristics of powder and superplasticizer large- ly affect the mortar property and so the proper water-Fig. 24 Dominance of gravel grading for flowability powder ratio and superplasticizer dosage cannot bethrough small spacing. fixed without trial mixing at this stage. Therefore, once
H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 11the mix proportion is decided, self-compactability has tobe tested by U-flow, slump-flow and funnel tests. Meth-ods for judging whether the water-powder ratio orsuperplasticizer dosage are larger or smaller than theproper value by using the test results, and methods forestimating the proper values are necessary. The relation-ships between the properties of the mortar in self-compacting concrete and the mix proportion have beeninvestigated and then formulated. These formulae canbe used to establish a rational method for adjusting thewater-powder ratio and superplasticizer dosage toachieve appropriate deformability and viscosity (Ouchi1998).3.3 Acceptance test at job site Fig. 25 Automatic acceptance test at job site.Since the degree of compaction in a structure mainlydepends on the self-compactability of concrete, andpoor self-compactability cannot be compensated by the There have been many examples of the developmentconstruction work, self-compactability must be checked of new type of superplasticizer for self-compacting con-for the whole amount of concrete just before casting at crete. Characterization of the dispersing effect ofthe job site. However, conventional testing methods for superplasticizer independent of the effect of water flowself-compactability require sampling and this can be is indispensable.extremely laborious if the self-compactability accep- The authors found that the ratio of G m to Rm wastance test is to be carried out for the whole amount of almost constant with the variety of Vw/Vp (volume ratioconcrete. A suitable acceptance test method for self- of water to powder) on condition that Sp/P was constantcompactability has been developed by Ouchi et al (Fig. 26). G m/Rm, the ratio of G m to Rm was proposed(1999).: as the index for the dispersing effect by superplasticizer (Fig. 27). The relationship between Sp/P and its effect (1) The testing apparatus is installed between the G m/Rm is quite different depending on the combination agitator truck and the pump at the job site. The whole amount of concrete is poured into the appara- tus. (2) If the concrete flows through the apparatus, the concrete is considered as self-compactable for the structure. If the concrete is stopped by the apparatus, the concrete is considered as having insufficient self- compactability and the mix proportion has to be adjusted. This apparatus was successfully used at the construc-tion site of the Osaka Gas LNG tank and saved a consid-erable amount of acceptance test work (Fig. 25)(Kitamura 1999). Fig. 26 Relationship between flow area and funnel speed of fresh mortar with variety of water-powder ratio3.4 New type of superplasticizer suitable for and superplasticizer dosage.Self-Compacting ConcreteThere is more room for improvement for admixturessuch as superplasticizer suitable for self-compactingconcrete. In order to achieve this purpose, characteriza-tion of materials is indispensable.The requirements for superplasticizer in self-compactingconcrete are summarized below. (1) High dispersing effect for low water/powder (cement) ratio: less than approx. 100% by volume (2) Maintenance of the dispersing effect for at least two hours after mixing (3) Less sensitivity to temperature changes Fig. 27 Definition of dispersing effect by superplasticizer by using flow and funnel test results.
12 H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003Fig. 28 Relationship between superplasticizer dosageand its effect in accordance with material in use. Fig. 29 Shin-kiba Ohashi bridge.of superplasticizer and powder material in use (Fig. 28)(Ouchi et al. 2001; Sugamata et al. 2001). At this stage,the relationship cannot be estimated without any experi- in confined zones where vibrating compaction is dif-mental result due to the chemical effect of super- ficultplasticizer depending on the combination to the powder (3) To eliminate noise due to vibration: effectivematerial in use. especially at concrete products plants3.5 Segregation-inhibiting agent The volume of self-compacting concrete in Japan isIt has been found that it is possible to manufacture self- shown in Fig. 30. The production of self-compactingcompacting concrete with constant quality, especially concrete as a percentage of Japanese ready-mixed con-self-compactability. However, any variation in material crete, which accounts for 70% of total concrete produc-characteristics can affect self-compactability. The most tion in Japan, is only 0.1%. The current status of self-influential variant is the water content of fine aggregate, compacting concrete is “special concrete” rather thanwhich results in variations in the water content of the “standard concrete.”concrete itself. To solve this problem, some general con- Other applications of self-compacting concrete arestruction companies employ a segregation-inhibiting summarized below.agent. This type of agent is effective in making self-compactability less sensitive to the variation of the Bridge (anchorage, arch, beam, girder, tower, pier,water content in the concrete. Various agents are avail- joint between beam & girder)able for this purpose in Japan (Hibino 1998). Box culvert Building4. Applications of Self-Compacting Concrete in Concrete filled steel columnJapan Tunnel (lining, immersed tunnel, fill of survey4.1 Current condition on application of self- tunnel)compacting concrete in Japan Dam (concrete around structure)After the development of the prototype of self- Concrete products (block, culvert, wall, water tank,compacting concrete at the University of Tokyo, inten- slab, and segment)sive research was begun in many places, especially inthe research institutes of large construction companies.As a result, self-compacting concrete has been used inmany practical structures. The first application of self-compacting concrete was in a building in June 1990.Self-compacting concrete was then used in the towers ofa prestressed concrete cable-stayed bridge in 1991 (Fig.29). Lightweight self-compacting concrete was used inthe main girder of a cable-stayed bridge in 1992. Sincethen, the use of self-compacting concrete in actual struc-tures has gradually increased. Currently, the main rea-sons for the employment of self-compacting concretecan be summarized as follows. (1) To shorten construction period (2) To assure compaction in the structure: especially Fig. 30 Volume of SCC cast in Japan.
H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 13 Diaphragm wall In addition, a rational acceptance test for self- Tank (side wall, joint between side wall and slab) compactability at the job site was newly introduced. Pipe roof The concrete casting was completed in June 1998.4.2 Large scale construction 4.3 Concrete productsSelf-compacting concrete is currently being employed Self-compacting concrete is often employed in concretein various practical structures in order to shorten the products to eliminate vibration noise (Fig. 32). Thisconstruction period of large-scale constructions. improves the working environment at plants and makes The anchorages of Akashi-Kaikyo (Akashi Straits) the location of concrete products plants in urban areasBridge opened in April 1998, a suspension bridge with possible. In addition, the use of self-compacting con-the longest span in the world (1,991 meters), is a typical crete extends the lifetime of mould for concrete prod-example (Fig. 31) (Kashima 1999). Self-compacting ucts (Uno 1999). The production of concrete productsconcrete was used in the construction of the two anchor- using self-compacting concrete has been graduallyages of the bridge. A new construction system that increasing (Fig. 33).makes full use of the performance of self-compactingconcrete was introduced for this purpose. The concrete 4.4 Necessity for new structural design andwas mixed at the batcher plant next to the site, and was construction systemsthen pumped out of the plant. It was transported 200 Using self-compacting concrete saves the cost of vibrat-meters through pipes to the casting site, where the pipes ing compaction and ensures the compaction of the con-were arranged in rows 3 to 5 meters apart. The concrete crete in the structure. However, total construction costwas cast from gate valves located at 5-meter intervals cannot always be reduced, except in large-scale con-along the pipes. These valves were automatically con- structions. This is because conventional constructiontrolled so that the surface level of the cast concrete systems are essentially designed based on the assump-could be maintained. The maximum size of the coarse tion that vibrating compaction of concrete is necessary.aggregate in the self-compacting concrete used at this Self-compacting concrete can greatly improve con-site was 40 mm. The concrete fell as much as 3 meters, struction systems previously based on conventionalbut segregation did not occur, despite the large size ofcoarse aggregate. In the final analysis, the use of self-compacting concrete shortened the anchorage construc-tion period by 20%, from 2.5 to 2 years. Self-compacting concrete was used for the wall of alarge LNG tank belonging to the Osaka Gas Company.The adoption of self-compacting concrete in this partic-ular project had the following merits. (1) The number of lots decreased from 14 to 10 as the height of one lot of concrete was increased. (2) The number of concrete workers was reduced from 150 to 50. (3) The construction period of the structure decreased from 22 months to18 months. Fig. 32 Casting of SCC for Tunnel Segment. Fig. 31 Anchorage 4A of Akashi-Kaikyo bridge. Fig. 33 Volume of SCC for concrete products in Japan.
14 H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 lished. In addition, new structural design and construc- tion systems making full use of self-compacting con- crete should be introduced. When self-compacting concrete becomes so widely used that it is seen as the “standard concrete” rather than a “special concrete,” we will have succeeded in creating durable and reliable concrete structures that require very little maintenance work. References Gagne, R., Pigeon, M., and Aïtcin, P. C. (1989). “Deicer salt scaling resistance of high performance concrete.” Paul Klieger Symposium on Performance of Con- crete, SP-122, ACI.Fig. 34 New construction system achieved by making Hayakawa, M., Matsuoka, Y., and Shindoh, T. (1993).full use of SCC (Proposed by Ozawa). “Development & application of super workable con- crete.” RILEM International Workshop on Specialconcrete that required vibrating compaction. This sort Concretes: Workability and Mixing.of compaction, which can easily cause segregation, has Hibino, M., Okuma, M., and Ozawa, K. (1998). “Rolebeen an obstacle to the rationalization of construction of viscosity agent in self-compactability of fresh con-work. Once this obstacle is eliminated, concrete con- crete.” Proceedings of the Sixth East-Asia Confer-struction can be rationalized and a new construction sys- ence on Structural Engineering & Construction, 2,tem, including formwork, reinforcement, support and 1313-1318.structural design, can be developed (Fig. 34). Kashima, S., Kanazawa, K., Okada, R., and Yoshikawa, One example of this is the so-called sandwich- S. (1999). “Application of self-compacting concretestructure, where concrete is filled into a steel shell. made with low-heat cement for bridge substructuresSuch a structure has already been completed in Kobe, of Honshu-Shikoku Bridge Authority.” Proceedingsand could not have been achieved without the develop- of the International Workshop on Self-Compactingment of self-compacting concrete (Fig. 35) (Shishido et Concrete, 255-261.al. 1999). Kitamura, H., Nishizaki, T., Ito, H., Chikamatsu, R., Kamada, F., and Okudate, M. (1999). “Construction5. Conclusions of prestressed concrete outer tank for LNG storage using high-strength self-compacting concrete.”Since a rational mix-design method and an appropriate Proceedings of the International Workshop on Self-acceptance testing method at the job site have both Compacting Concrete, 262-291.largely been established for self-compacting concrete, Maekawa, K., and Ozawa, K. (1999). “Development ofthe main obstacles for the wide use of self-compacting SCC’s prototype.” (written in Japanese), Self-concrete can be considered to have been solved. The Compacting High-Performance Concrete, Socialnext task is to promote the rapid diffusion of the tech- System Institute, 20-32.niques for the production of self-compacting concrete Nagamoto, N., and Ozawa, K. (1997). “Mixture propor-and its use in construction. Rational training and quali- tions of self-compacting high performance concrete,”fication systems for engineers should also be estab- ACI International, SP-172, 623-636. Okamura, H., Maekawa, K., and Ozawa, K. (1993). “High Performance Concrete.” Gihodo Publishing. Okamura, H. and Ozawa, K. (1995). “Mix-design for self-compacting concrete.” Concrete Library of JSCE, 25, 107-120. Ouchi, M., Hibino, M., Ozawa, K.. and Okamura, H. (1998). “A rational mix-design method for mortar in self-compacting concrete.” Proceedings of the Sixth East Asia-Pacific Conference on Structural Engi- neering & Construction, 2, 1307-1312. Ouchi, M. (1999). “State-of-the-art report on self- compactability evaluation.” Proceedings of the Inter- national Workshop on Self-Compacting Concrete (CD-ROM). Also available from Concrete Engineer- ing Series, 30, JSCE. Ouchi, M. and Edamatsu, Y. (2000). “A Simple evalua- Fig. 35 Sandwich structure for immersed tunnel. tion method for interaction between coarse aggregate
H. Okamura and M. Ouchi / Journal of Advanced Concrete Technology Vol. 1, No. 1, 5-15, 2003 15 and mortar particles in self-compacting concrete.” Kume, H. (1999). “Pouring works of high fluidity Transaction of JCI. concrete for immersed tunnel by steel-concrete com-Ouchi, M., Hibino, M., Sugamata, T., and Okamura, H. posite structure.” Proceedings of the International (2001). “A quantitative evaluation method for the Workshop on Self-Compacting Concrete, 328-346. effect of superplasticizer in self-compacting Sugamata, T., Hibino, M., Ouchi, M., and Okamura, H. concrete”, Transactions of JCI, 15-20. ( 2 0 0 1 ) . “ E ff e c t s o f m o l e c u l a r s t r u c t u r e s o fOzawa, K., Maekawa, K., Kunishima, M., and polycarboxylate polymers on cement particles Okamura, H. (1989). “Development of high perfor- dispersibility.” Concrete Library International, 38, mance concrete based on the durability design of JSCE. concrete structures”, Proceedings of the second East- Uno, Y. (1999). “State-of-the art report on concrete Asia and Pacific Conference on Structural Engineer- products made of SCC,” Proceedings of the Interna- ing and Construction (EASEC-2), 1, 445-450. tional Workshop on Self-Compacting Concrete, 262-Shishido, T., Shiraiwa, S., Ishii, J., Yamamoto, S., and 291.